Spreadsheet: 2356dacc-60fb-41cd-9075-114092c0521a
Sheet: 1. Structural

 |  |  |  |  |  |  | MD-SLS; Part of SOP
M-spec |  | Linked standards |  | Material / Grade | Steel Quality Level | Product | Dimension limitation | Certificate | Delivered cond. | Chemical composition |  |  |  |  |  |  |  |  | Tensile |  |  |  |  |  |  |  |  |  |  |  |  |  | Impact testing |  |  |  |  |  |  |  |  |  |  |  | Hardness (maxim) | Micro-structure examin | Surface condition |  | Suitability for hot dip galvanizing
 |  |  |  |  |  |  |  |  |  | Cast / Ladle analysis |  | Residual elements and other comments |  | Product analysis |  | CEV / Pcm |  |  | Minimum yield strength |  |  | [NAME] strength |  |  |  |  | Yield/Tensile-ratio |  | Elongation (minimum) |  |  |  | Longitudinal: J (ft-lb) |  |  |  |  |  |  |  | Transverse J
 | rev. | NORSOK | Other |  |  |  |  |  |  | Main elements |  |  |  | Main elements |  |  |  |  | Dimension m m | KSI | MPa | Dimension m m | KSI | MPa | Through thickness (t>25mm) |  | Dim. m m | % | Dim. / cond. | [NAME]. % | Transv. % | Red. of area % | Temp ºC (ºF) | Normal sample size (10mmx10mm) |  |  | Mid. Thickn. | Reduced sample size |  |  | Temp ºC (ºF) | Dim  / Cond | Average | Single
 |  |  |  |  |  |  | m m |  |  | Element | Content % | Element | Content % | Element | Content % | Dim | CEV | Pcm |  |  |  |  |  |  | KSI | MPa |  |  |  |  |  |  |  | Dim  / Cond | Average | Single |  | Sample dimensions | Average | Single
M10003 | J | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355K2H (FF) | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished welded or seamless hollow tubulars | seamless hollow sections: [NAME]  welded hollow sections: t<20[NAME] | EN 10204 Type 3.1 or higher | Delivery condition for EN 10210-1 S355K2H and –J2H hot finished  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Chromium Nickel Molybdenum Copper | [NAME] 0.55 [NAME] 1.60 max 0.030 [NAME] 0.030 reported reported reported reported reported reported | Al | If sufficient N binding elements are present, the minimum Al content does not apply. | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.60 max 1.70 max 0.040 max 0.040 reported reported reported reported reported reported |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 | [NAME] 3<t<40 | 68-91 | 510 - 680 470 - 630 |  |  |  |  | 5,65√S0 4√S0 | 22 25 | 20 23 |  | -20 |  | 40 | 28 |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1
M10003 | J | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355NH (GF) | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished welded or seamless hollow tubulars | seamless hollow sections: [NAME]  welded hollow sections: t<20[NAME] | EN 10204 Type 3.1 or higher | Delivery condition for EN 10210-1 S355NH is normalized, (N). | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Titanium Chromium Nickel Molybdenum Copper Nitrogen Aluminium tot | [NAME] 0.50 0.90 - 1.65 [NAME] 0.035  [NAME] 0.030  [NAME] 0.050 [NAME] 0.12 max 0.03 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 [NAME] 0.35 max 0.020  min 0.020 |  |  | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Titanium Cromium Nickel Molybdenum Copper Nitrogen Aluminium tot | [NAME] 0.55 0.85 - 1.75 max 0.040  [NAME] 0.035  [NAME] 0.060 [NAME] 0.14 max 0.04 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.022 min 0.015 |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 | 3<t<40 | 68-91 | 470 - 630 |  |  |  |  | 5,65√S0 4√S0 | 22 25 | 20 23 |  | -20 |  | 40 | 28 |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1.
M10003 | J | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355J2H (FF) | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubulars | [NAME] | EN 10204 Type 3.1 or higher | Delivery condition for EN 10210-1 S355K2H and –J2H hot finished  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Chromium Nickel Molybdenum Copper | [NAME] 0.55 [NAME] 1.60 max 0.030 [NAME] 0.030 reported reported reported reported reported reported | Al | If sufficient N binding elements are present, the minimum Al content does not apply. | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.60 max 1.70 max 0.040 max 0.040 reported reported reported reported reported reported |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 | [NAME] 3<t<40 | 68-91 | 510 - 680 470 - 630 |  |  |  |  | 5,65√S0 4√S0 | 22 25 | 20 23 |  | -20 |  | 40 | 28
M10003 | I | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355K2H | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubulars  -seamless -welded | seamless hollow sections: [NAME]  welded hollow sections: t<20[NAME] | EN 10204 Type 3.1 or higher | Hot finished.  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.55 [NAME] 1.60 max 0.030 [NAME] 0.030 reported reported reported reported reported reported |  |  | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.60 max 1.70 max 0.040 max 0.040 reported reported reported reported reported reported |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 | [NAME] 3<t<40 | 68 - 91 | 510 - 680 470 - 630 |  |  |  |  |  | 22 | 20 |  | -20 |  | 40 | 28
M10003 | I | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355NH | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubulars  -seamless -welded | seamless hollow sections: [NAME]  welded hollow sections: t<20[NAME] | EN 10204 Type 3.1 or higher | Delivery condition for EN 10210-1 S355NH is normalized, (N). | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Titanium Cromium Nickel Molybdenum Copper Nitrogen Aluminium tot | [NAME] 0.50 0.90 - 1.65 [NAME] 0.035  [NAME] 0.030  [NAME] 0.050 [NAME] 0.12 max 0.03 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 [NAME] 0.35 max 0.020  min 0.020 |  |  | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Titanium Cromium Nickel Molybdenum Copper Nitrogen Aluminium tot | [NAME] 0.55 0.85 - 1.75 max 0.040  [NAME] 0.035  [NAME] 0.060 [NAME] 0.14 max 0.04 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.022 min 0.015 |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 |  | 68 - 91 | 470 - 630 |  |  |  |  |  | 22 | 20 |  | -20 |  | 40 | 28
M10003 | I | NORSOK M120 Y-07, rev 3 06/07 | EN 10210-1 | S355J2H | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubulars | t<16mm | EN 10204 Type 3.1 or higher | Hot finished.  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.55 [NAME] 1.60 max 0.030 [NAME] 0.030  reported reported reported reported reported reported |  |  | Carbon Silicon Manganese Phosphorus Sulfur Vanadium Titanium Cromium Nickel Molybdenum Copper | [NAME] 0.60 max 1.70 max 0.040 max 0.040  reported reported reported reported reported reported |  | [NAME] 0.43 |  | t<16 16<t<40 | 51 50 | 355 345 | [NAME] 3<t<40 | 68 - 91 | 510 - 680 470 - 630 |  |  |  |  |  | 22 | 20 |  | -20 | [NAME] | 40 | 28
M10004 | I | M120 Y-05, rev 3 06/07 | EN 10025-2 | S355J2 | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | one of following:  Normalized/normalized rolled (N)  Thermomechanically rolled (M)  As Rolled (AR) | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  max 0.55 [NAME] 1.60 max 0.025 [NAME] 0.025 max 0.55 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  [NAME] 0.60 max 1.70 [NAME] 0.035 [NAME] 0.035 [NAME] 0.60 |  | [NAME] 0.43 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t<3 t>3 | 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28
M10004 | I | M120 Y-05, rev 3 06/07 | EN 10025-2 | S355K2 | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | one of following:  Normalized/normalized rolled (N)  Thermomechanically rolled (M)  As Rolled (AR) | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  max 0.55 [NAME] 1.60 max 0.025 [NAME] 0.025 max 0.55 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  [NAME] 0.60 max 1.70 [NAME] 0.035 [NAME] 0.035 [NAME] 0.60 |  | [NAME] 0.43 |  | 6-16mm 16-40mm 40-50mm | 51 | 355 345 335 |  | 68 - 91 | 470 - 630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28
M10004 | I |  | DNV OS B101 | NV E36 |  | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | CR: Controlled rolled  N: Normalised  QT: Quenched & Tempered  TM Thermo-mechanically rolled | C Si Mn P S Cu Cr Ni Mo Al ac. sol Al tot Nb V Ti | [NAME] 0.16 0.10 - 0.50 0.9 - 1.6 max 0.035 [NAME] 0.035 [NAME] 0.35 max 0.20 max 0.40 0.08 0.015 - 0.08 0.020 - 0.085 0.02 - 0.05 0.05 - 0.10 0.02 |  |  |  |  |  | [NAME] 0.38 |  |  | 51 | 355 |  | 68-91 | 470-630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28 |  |  |  |  | -40 |  | 24 | 16.8
M10004 | I |  | DNV OS B101 | NV EW36 |  | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | CR: Controlled rolled  N: Normalised  QT: Quenched & Tempered  TM Thermo-mechanically rolled | C Si Mn P S Cu Cr Ni Mo Al tot Nb V Ti N B Nb+V Nb+V+Ti | [NAME] 0.12 0.10 - 0.50 0.90 - 1.60 max 0.020 [NAME] 0.008 [NAME] 0.35 max 0.20 [NAME] 0.70 [NAME] 0.08 max 0.06 [NAME] 0.04 max 0.06 [NAME] 0.05 [NAME] 0.010 [NAME] 0.0005 max 0.06 [NAME] 0.10 | As Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03 max 0.01 max 0.02 max 0.01 max 0.01 max 0.005 30ppm - if agreed  min 2:1 |  |  |  | [NAME] 0.43 | [NAME] 0.22 | <25mm 25-50mm | 51 | 355 335 |  | 68-91 | 470-630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28 | 35 |  |  |  | -40 |  | 50 | 35
M10004 | G | M120 Y-05, rev 3 06/07 | EN 10025-2 | S355J2 | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | one of following:  Normalized/normalized rolled (N)  Thermomechanically rolled (M)  As Rolled (AR) | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  max 0.55 [NAME] 1.60 max 0.025 [NAME] 0.025 max 0.55 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  [NAME] 0.60 max 1.70 [NAME] 0.035 [NAME] 0.035 [NAME] 0.60 |  | [NAME] 0.43 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t<3 t>3 | 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28
M10004 | G | M120 Y-05, rev 3 06/07 | EN 10025-2 | S355K2 | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | one of following:  Normalized/normalized rolled (N)  Thermomechanically rolled (M)  As Rolled (AR) | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  max 0.55 [NAME] 1.60 max 0.025 [NAME] 0.025 max 0.55 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Copper | [NAME] 0.16  [NAME] 0.60 max 1.70 [NAME] 0.035 [NAME] 0.035 [NAME] 0.60 |  | [NAME] 0.43 |  | 6-16mm 16-40mm 40-50mm | 51 | 355 345 335 |  | 68 - 91 | 470 - 630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28
M10004 | G |  | DNV OS B101 | NV E36 |  | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | CR: Controlled rolled  N: Normalised  QT: Quenched & Tempered  TM Thermo-mechanically rolled | C Si Mn P S Cu Cr Ni Mo Al ac. sol Al tot Nb V Ti | [NAME] 0.16 0.10 - 0.50 0.9 - 1.6 max 0.035 [NAME] 0.035 [NAME] 0.35 max 0.20 max 0.40 0.08 0.015 - 0.08 0.020 - 0.085 0.02 - 0.05 0.05 - 0.10 0.02 |  |  |  |  |  | [NAME] 0.38 |  |  | 51 | 355 |  | 68-91 | 470-630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28 |  |  |  |  | -40 |  | 24 | 16.8
M10004 | G |  | DNV OS B101 | NV EW36 |  | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher | CR: Controlled rolled  N: Normalised  QT: Quenched & Tempered  TM Thermo-mechanically rolled | C Si Mn P S Cu Cr Ni Mo Al tot Nb V Ti N B Nb+V Nb+V+Ti | [NAME] 0.12 0.10 - 0.50 0.90 - 1.60 max 0.020 [NAME] 0.008 [NAME] 0.35 max 0.20 [NAME] 0.70 [NAME] 0.08 max 0.06 [NAME] 0.04 max 0.06 [NAME] 0.05 [NAME] 0.010 [NAME] 0.0005 max 0.06 [NAME] 0.10 | As Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03 max 0.01 max 0.02 max 0.01 max 0.01 max 0.005 30ppm - if agreed  min 2:1 |  |  |  | [NAME] 0.43 | [NAME] 0.22 | <25mm 25-50mm | 51 | 355 335 |  | 68-91 | 470-630 |  |  |  |  | 3<t<40   t>40 | 22   21 | 20   19 |  | -20 |  | 40 | 28 | 35 |  |  |  | -40 |  | 50 | 35
 |  |  | EN 10025-3 | S355N | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  [NAME] 0.50 0.90 - 1.65 [NAME] 0.030 [NAME] 0.025 max 0.05 max 0.12 min 0.02 max 0.05 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 max 0.55 max 0.015 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  max 0.55 0.85 - 1.75 [NAME] 0.035 [NAME] 0.030 max 0.06 [NAME] 0.14 min 0.015 max 0.06 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.60 max 0.017 |  | [NAME] 0.43 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t>3 | 68 - 91 | 470 - 630 |  |  |  |  |  | 22 |  |  | -20 |  | 40 | 28
 |  |  | EN 10025-3 | S355NL | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  [NAME] 0.50 0.90 - 1.65 max 0.025 max 0.020 [NAME] 0.05 max 0.12 min 0.02 max 0.05 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 max 0.55 max 0.015 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  max 0.55 0.85 - 1.75 [NAME] 0.030 [NAME] 0.025 max 0.06 [NAME] 0.14 min 0.015 max 0.06 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.60 max 0.017 |  | [NAME] 0.43 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t>3 | 68 - 91 | 470 - 630 |  |  |  |  |  | 22 |  |  | -20 -30 -40 -50 |  | 47 40 31 27 | 32.9 28 21.7 18.9
 |  |  | EN 10025-4 | S355M | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.14 [NAME] 0.50 [NAME] 1.60 max 0.030  [NAME] 0.025  max 0.05 [NAME] 0.10 min 0.02 max 0.05 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 max 0.55 max 0.015 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  max 0.55 0.85 - 1.75 [NAME] 0.035 [NAME] 0.030 max 0.06 [NAME] 0.14 min 0.015 max 0.06 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.60 max 0.017 | [NAME] [NAME] | [NAME] 0.40 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t<40 t>40 | 68 - 91 | 470 - 630 450 - 610 |  |  |  |  |  | 22 |  |  | -20 |  | 40 | 28
 |  |  | EN 10025-4 | S355ML | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.14 [NAME] 0.50 [NAME] 1.60 max 0.25 [NAME] 0.20 max 0.05 [NAME] 0.10 min 0.02 max 0.05 [NAME] 0.30 [NAME] 0.50 [NAME] 0.10 max 0.55 max 0.015 |  |  | Carbon  Silicon: Manganese: Phoshorus: Sulfur: Nb V Al tot Ti Cr Ni Mo Copper N | [NAME] 0.16  max 0.55 0.85 - 1.75 [NAME] 0.030 [NAME] 0.025 max 0.06 [NAME] 0.14 min 0.015 max 0.06 [NAME] 0.35 max 0.55 [NAME] 0.13 [NAME] 0.60 max 0.017 | [NAME] [NAME] | [NAME] 0.40 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t<40 t>40 | 68 - 91 | 470 - 630 450 - 610 |  |  |  |  |  | 22 |  |  | -20 -30 -40 -50 |  | 47 40 31 27 | 32.9 28 21.7 18.9
 |  |  | EN 10025-5 | S355K2W | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates Sections | t<50[NAME] | EN 10204 Type 3.1 or higher |  | Carbon  Silicon: Manganese: Phoshorus: (-long product) Sulfur: (-long product) Cr Copper Ni Mo Zr N binding elem: Al Nb V Ti | [NAME] 0.16 [NAME] 0.50 0.50 - 1.50 [NAME] 0.030 ([NAME] 0.035) [NAME] 0.030 ([NAME] 0.035) 0.40 - 0.80 0.25 - 0.55 max 0.65 [NAME] 0.30 [NAME] 0.15  min 0.020 0.015 - 0.060 0.02 - 0.12 0.02 - 0.10 |  |  | Carbon  Silicon: Manganese: Phoshorus: (-long product) Sulfur: (-long product) Cr Copper Ni Mo Zr N binding elem: Al Nb V Ti | [NAME] 0.16 max 0.55 0.45 - 1.60 max 0.035 ([NAME] 0.040) [NAME] 0.035 ([NAME] 0.040) 0.35 - 0.85 0.20 - 0.60 [NAME] 0.70 [NAME] 0.35 max 0.17  min 0.020 0.015 - 0.060 0.02 - 0.12 0.02 - 0.10 |  | [NAME] 0.43 |  | t<16 16<t<40 t>40 | 51 | 355 345 335 | t<3  flat product 3<t<12 long product 3<t<50 | 68 - 91 | 510 - 680   470 - 630 |  |  |  |  | [NAME]1.5<t<2 2<t<2.5 2.5<t<3  L0=5.65√S0 3<t<40 t>40 | 16 17 18   22 21 | 14 15 16   20 19 |  | -20 |  | 40 | 28
M10005 | H | NOROSK M120 Y-06, rev 3 06/07 | EN 10225 | S355G1+N | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished seamless tubulars | [NAME] | EN 10204 Type 3.1 or higher | Normalized/normalized rolled (N) | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium tot Copper Nitrogen Niobium Titanium  Vanadium Nb+V | [NAME] 0.16  [NAME] 0.50 0.90-1.65 [NAME] 0.035 [NAME] 0.030 [NAME] 0.30 [NAME] 0.10 [NAME] 0.50  min. 0.02 [NAME] 0.35 [NAME] 0.015 [NAME] 0.050 [NAME] 0.030 max 0.120 max 0.10 | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  min 2:1 | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium tot Copper Nitrogen Niobium Titanium  Vanadium | [NAME] 0.16  [NAME] 0.60 0.85-1.75 max 0.040 [NAME] 0.035 [NAME] 0.35 [NAME] 0.13 max 0.55  min. 0.015 max 0.354 max 0.017 [NAME] 0.060 [NAME] 0.031 [NAME] 0.140 |  | [NAME] 0.43 |  | 6<t<16 16<t<40 | 51 50 | 355 345 |  | 68-91 | 470 - 630 |  |  |  | 0.87 | 5,65√S0 4√S0 | 22 25 |  |  | -20 (-4) |  | 50 (35) | 38 (26.25) |  | 10mmx7.5mm 10mmx5mm | 37,5 25 | 28,5 19 |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1.
M10005 | F | NOROSK M120 Y-06, rev 3 06/07 | EN 10225 | S355G1+N | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished seamless tubulars | [NAME] | EN 10204 Type 3.1 or higher | Normalized/normalized rolled (N) | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium tot Copper Nitrogen Niobium Titanium  Vanadium Nb+V | [NAME] 0.16  [NAME] 0.50 0.90-1.65 [NAME] 0.035 [NAME] 0.030 [NAME] 0.30 [NAME] 0.10 [NAME] 0.50  min. 0.02 [NAME] 0.35 [NAME] 0.015 [NAME] 0.050 [NAME] 0.030 max 0.120 max 0.10 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium tot Copper Nitrogen Niobium Titanium  Vanadium | [NAME] 0.16  [NAME] 0.60 0.85-1.75 max 0.040 [NAME] 0.035 [NAME] 0.35 [NAME] 0.13 max 0.55  min. 0.015 max 0.354 max 0.017 [NAME] 0.060 [NAME] 0.031 [NAME] 0.140 |  | [NAME] 0.43 |  | 6<t<16 16<t<40 | 51 50 | 355 345 |  | 68 - 91 | 470 - 630 |  |  |  | 0.87 | 5,65√S0 4√S0 | 22 25 |  |  | -20 (-4) |  | 50 (35) | 37.5 (26.25)
M10006 | D | NORSOK M120 Y27, rev 4 06/07 | EN 10225 | S355G14+Q  S355G14+N | SQL II  S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Seamless tubulars and hollow sections |  | EN 10204 Type 3.1 or higher | S355G14+Q: Quenched and tempered (Q or QT)  S355G14+N: Normalized / normalized rolled (N) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  Ti   V Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,6 max 0,025 [NAME] 0,25 [NAME] 0,3 min 0,06 max 0,35 [NAME] 0,014 max 0,05 [NAME] 0,02 max 0,10 max 0,8 max 0,1 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  min 2:1 (exept when other N-binding elements are used) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  Ti   V Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,6 max 0,025 [NAME] 0,25 [NAME] 0,3 min 0,06 max 0,35 [NAME] 0,014 max 0,05 [NAME] 0,02 max 0,10 max 0,8 max 0,1 [NAME] |  | [NAME] 0.43 |  | t<20 20<t<40 | 51 50 | 355 345 |  | 67-90 | 460 - 620 |  |  |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 | 35 |  | 10mmx7.5mm 10mmx5mm | 37,5 25 | 26,25 17,5
M10006 | B | NORSOK M120 Y27, rev 4 06/07 | EN 10225 | S355G14+Q  S355G14+N | SQL II  S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Seamless tubulars and hollow sections |  | EN 10204 Type 3.1 or higher | S355G14+Q: Quenched and tempered (Q or QT)  S355G14+N: Normalized / normalized rolled (N) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  Ti   V Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,6 max 0,025 [NAME] 0,25 [NAME] 0,3 [NAME] 0,06 [NAME] 0,014 max 0,05 [NAME] 0,02 max 0,10 max 0,8 max 0,1 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  Ti   V Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,6 max 0,025 [NAME] 0,25 [NAME] 0,3 [NAME] 0,06 [NAME] 0,014 max 0,05 [NAME] 0,02 max 0,10 max 0,8 max 0,1 [NAME] |  | [NAME] 0.43 |  | t<20 20<t<40 |  | 355 345 |  | 67 - 90 | 460 - 620 |  |  |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 | 35
M10008 | D | M120 Y28,  rev 3 06/07 | EN 10225 | S355G13+N | SQL II  S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Welded tubulars and hollow sections | t<20[NAME] | EN 10204 Type 3.1 or higher | Normalized/normalized rolled (N) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  V  Ti  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,60 [NAME] 0,025 max 0,015 max 0,25 [NAME] 0,060 [NAME] 0,014 max 0,050 [NAME] 0,100 max 0,020 max 0,80 max 0,10 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  min 2:1 (exept when other N-binding elements are used) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  V  Ti  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,60 [NAME] 0,025 max 0,015 max 0,25 [NAME] 0,060 [NAME] 0,014 max 0,050 [NAME] 0,100 max 0,020 max 0,80 max 0,10 [NAME] |  | [NAME] 0.43 |  | <20mm | 51 | 355 |  | 67-90 | 460 - 620 |  |  |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 (35) | 35 (24,5) |  | 10mmx7.5mm 10mmx5mm | 37,5 25 | 26,5 17,5 |  |  |  |  |  | x | Hollow sections shall be suitable for use as primary components
M10008 | B | M120 Y28, rev 3 06/07 | EN 10225 | S355G13+N | SQL II  S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Welded tubulars and hollow sections | t<20[NAME] | EN 10204 Type 3.1 or higher | Normalized / normalized rolled (N) | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  V  Ti  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,60 [NAME] 0,025 max 0,015 max 0,25 [NAME] 0,060 [NAME] 0,014 max 0,050 [NAME] 0,100 max 0,020 max 0,80 max 0,10 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  Si Mn P  S  Cr Mo Ni  Al (total) Cu  N  Nb  V  Ti  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,60 [NAME] 0,025 max 0,015 max 0,25 [NAME] 0,060 [NAME] 0,014 max 0,050 [NAME] 0,100 max 0,020 max 0,80 max 0,10 [NAME] |  | [NAME] 0.43 |  | <20mm | 51 | 355 |  | 67 - 90 | 460 - 620 |  |  |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 (35) | 35 |  |  |  |  |  |  |  |  |  | x
M10010 | E | M120 Y-01, rev 5 06/07 | EN 10025-2 | S235JR (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized/normalized rolled (N) or As Rolled (AR) | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.17 [NAME] 1.40 [NAME] 0.035 [NAME] 0.035 [NAME] 0.012 max 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.19 [NAME] 1.50 [NAME] 0.045 [NAME] 0.045 [NAME] 0.014 [NAME] 0.60 |  | [NAME] 0.35 |  | t ≤ 16  16<t ≤ 25 | 34 32.5 | 235 225 |  | 52 - 74 | 360 - 510 |  |  |  |  | ≥3 t ≤ 40 5,65√S0 4√S0   <1mm <1.5mm <2mm <2.5mm <3mm >3mm | 26  30   17 18 19 20 21 26 | 15 16 17 18 19 24 |  | 20 | Optional | 27 | 18.9
M10010 | E | M120 Y-01, rev 5 06/07 | EN 10210-1 | S235JRH (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Hot finished tubululars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished. seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.17 [NAME] 1.40 max 0.040 max 0.040 max 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.19 [NAME] 1.50 [NAME] 0.050 [NAME] 0.050 [NAME] 0.011 | t ≤ 16  16<t ≤ 25 | [NAME] 0.37 max 0.39 |  | t ≤ 16  16<t ≤ 25 | 34 32.5 | 235 225 |  | 52 - 74 | 360 - 510 |  |  |  |  | ≥3 t ≤ 40 5,65√S0 4√S0 | 26 30 | 24 27 |  | 20 | Optional | 27 | 18.9
M10010 | E | [NAME], rev 5 06/07 | EN 10219-1 | S235JRH (FF) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Cold formed tubulars | t<25mm | EN 10204 Type 2.2 or higher | cold formed | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.17 [NAME] 1.40 max 0.040 max 0.040 max 0.009 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.19 [NAME] 1.50 [NAME] 0.050 [NAME] 0.050 [NAME] 0.011 |  | [NAME] 0.35 |  | t ≤ 16  16<t ≤ 25 | 34 32.5 | 235 225 | [NAME] | 52 - 74 52 - 74 | 360 - 510 360 - 510 |  |  |  |  | ≥3 t ≤ 40 5,65√S0 4√S0  Other dim and shapes for 5,65√S0: D/T<15 (round) and (B+H)/2T<12.5 [NAME] | 24 27        22 17 | 22 25        20 15 |  | 20 | Optional | 27 | 18.9
M10010 | C | M120 Y-01, rev 5 07/07 | EN 10025-2 | S235JR | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized / normalized rolled (N)   or  As Rolled (AR) | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.17 [NAME] 1.40 [NAME] 0.035 [NAME] 0.035 [NAME] 0.012 max 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.19 [NAME] 1.50 [NAME] 0.045 [NAME] 0.045 [NAME] 0.014 [NAME] 0.60 |  | [NAME] 0.35 |  | <16mm >16mm | 34 32.5 | 235 225 |  | 52 - 74 | 360 - 510 |  |  |  |  | >3mm 5,65√S0 4√S0  Other dim for 5,65√S0: <1mm <1.5mm <2mm <2.5mm <3mm | 26 30    17 18 19 20 21 | 24     15 16 17 18 19 |  | 20 | Optional | 27 | 18.9
M10010 | C | M120 Y-01, rev 5 07/07 | EN 10210-1 | S235JRH | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubululars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished.  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.17 [NAME] 1.40 max 0.040 max 0.040 max 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.19 [NAME] 1.50 [NAME] 0.050 [NAME] 0.050 [NAME] 0.011 | t<16 t>16 | [NAME] 0.37 max 0.39 |  | <16mm >16mm | 34 32.5 | 235 225 |  | 52 - 74 | 360 - 510 |  |  |  |  | t>3mm 5,65√S0 4√S0 | 26 30 | 24 27 |  | 20 | Optional | 27 | 18.9
M10010 | C | [NAME], rev 5 07/07 | EN 10219-1 | S235JRH | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars | t<25mm | EN 10204 Type 2.2 or higher | cold formed | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.17 [NAME] 1.40 max 0.040 max 0.040 max 0.009 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.19 [NAME] 1.50 [NAME] 0.050 [NAME] 0.050 [NAME] 0.011 |  | [NAME] 0.35 |  | <16mm >16mm | 34 32.5 | 235 225 | [NAME] | 52 - 74 52 - 74 | 360 - 510 360 - 510 |  |  |  |  | t>3mm 5,65√S0 4√S0  Other dim and shapes for 5,65√S0: D/T<15 (round) and (B+H)/2T<12.5 [NAME] | 24 27        22 17 | 22 25        20 15 |  | 20 | Optional | 27 | 18.9
M10011 | F | M120 Y02, rev 4 06/07 | EN 10025-2 | S275JR (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized/normalized rolled (N), Thermomechanically rolled (M) or As Rolled (AR) | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.21 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.012 max 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.24 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.014 [NAME] 0.60 |  | [NAME] 0.40 |  | <16mm 16<t ≤25[NAME] | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | t [NAME] 3mm 5,65√S0 4√S0 | 23 26 | 21 |  | 20 | Optional | 27 | 18.9 |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1
M10011 | F | M120 Y02, rev 4 06/7 | EN 10210-1 | S275J0H (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Hot finished tubululars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished. seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.20 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.22 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.011 | t ≤ 16   16< t ≤ 25 | [NAME] 0.41 [NAME] 0.43 |  | <16mm 16<t ≤25[NAME] | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | t [NAME] 3mm 5,65√S0 4√S0 | 23 26 | 21 |  | 0 | Optional | 27 | 18.9 |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1
M10011 | F | M120 Y02, rev 4 06/07 | EN 10219-1 | S275J0H (FF) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC | Cold formed tubulars | t<25mm | EN 10204 Type 2.2 or higher | cold formed | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.20 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.22 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.011 |  | [NAME] 0.40 |  | <16mm 16<t ≤25[NAME] | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | t>3mm 5,65√S0 4√S0  Other dim and shapes for 5,65√S0: D/T<15 (round) and B+H)/2T<12.5 | 20 23       18 |  |  | 0 | Optional | 27 | 18.9 |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1
M10011 | D | M120 Y02, rev 4 06/07 | EN 10025-2 | S275JR | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized/ normalized rolled (N  or  Thermomechanically rolled (M)   or  As Rolled (AR) | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.21 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.012 max 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.24 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.014 [NAME] 0.60 |  | [NAME] 0.40 |  | <16mm >16mm | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | >3mm 5,65√S0 4√S0  Other dim for 5,65√S0: <1mm <1.5mm <2mm <2.5mm <3mm | 23 26    15 16 17 18 19 | 21(24)     13 14 15 16 17 |  | 20 | Optional | 27 | 18.9
M10011 | D | M120 Y02, rev 4 | EN 10210-1 | S275J0H | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubululars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished  -seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.20 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.22 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.011 | t<16 t>16 | [NAME] 0.41 [NAME] 0.43 |  | <16mm >16mm | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | 5,65√S0 4√S0 | 23 26 | 21 |  | 0 | Optional | 27 | 18.9
M10011 | D | M120 Y02, rev 4 | EN 10219-1 | S275J0H | IV  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars | t<25mm | EN 10204 Type 2.2 or higher | cold formed | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.20 [NAME] 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon: Manganese: Phosphorus : Sulfur: [NAME]: | [NAME] 0.22 [NAME] 1.60 max 0.045 [NAME] 0.045 [NAME] 0.011 |  | [NAME] 0.40 |  | <16mm >16mm | 40 38.5 | 275 265 | [NAME] | 62 - 84 59 - 81 | 430 - 580 410 - 560 |  |  |  |  | t>3mm 5,65√S0 4√S0  Other dim and shapes for 5,65√S0: D/T<15 (round) and B+H)/2T<12.5 [NAME] | 20 23       18 17 |  |  | 0 | Optional | 27 | 18.9
M10012 | E | M120 Y-04,rev 2 06/07 | EN 10025-2 | S355J0 (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized/normalized rolled (N) Thermomechanically rolled (M) As Rolled (AR) | Carbon Silicon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.20  max 0.55 [NAME] 0.030 [NAME] 0.030 [NAME] 0.012 [NAME] 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon  Silicon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.23  [NAME] 0.60 max 1.70 max 0.040 max 0.040 max 0.014 [NAME] 0.60 |  | [NAME] 0.45 |  | t<16 16<t ≤25 | 51 50 | 355 345 | [NAME] | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | >3mm 5,65√S0 4√S0 | 22 25 | 20 23 |  | 0 (32) |  | 27 (20) | 19 (14) |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1.
M10012 | E | M120 Y-04, rev 2 06/07 | EN 10210-1 | [NAME] (FN) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubulars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished. seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.22 max 0.55 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Silicon Manganese Phosphorus: Sulfur: [NAME]: | [NAME] 0.25 [NAME] 0.60 max 1.70 [NAME] 0.045 [NAME] 0.045 [NAME] 0.011 | t ≤ 16 16< t ≤ 25 | [NAME] 0.45 [NAME] 0.47 |  | t<16 16<t<25 | 51 50 | 355 345 | [NAME] 3<t<25 | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | 5,65√S0 4√S0 | 22 25 | 20 23 |  | 0 (32) |  | 27 (20) | 19 (14) |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1.
M10012 | E | M120 Y-04, rev 2 06/07 | EN 10219-1 | S355J2H (FF) | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars | t<25mm | EN 10204 Type 3.1 | as rolled or normalized/normalized rolled (N) followed by cold forming. | Carbon Silicon Manganese Phosphorus Sulfur | [NAME] 0.22 max 0.55 [NAME] 1.60  max 0.030 [NAME] 0.030 |  |  | Carbon Silicon Manganese Phosphorus Sulfur | [NAME] 0.24 max 0.60 max 1.70 max 0.040 max 0.040 |  | [NAME] 0.45 |  | t<16 16<t<25 | 51 50 | 355 345 | [NAME] | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | t≥3[NAME]: 5,65√S0 4√S0   Other dim and shapes for 5,65√S0: D/T<15 (round) and B+H)/2T<12.5 | 20 23        18 |  |  | -20 (-4) |  | 27 (20) | 19 (14) |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1.
M10012 | C | M120 Y-04,rev 2 06/07 | EN 10025-2 | S355J0 | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher | Normalized/normalized rolled (N) Thermomechanically rolled (M) As Rolled (AR) | Carbon  Silicon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.20 (0.22 - cold roll forming) [NAME] 0.55 [NAME] 0.030 [NAME] 0.030 [NAME] 0.012 max 0.55 | N: | Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon  Silicon Manganese Phosphorus Sulfur Nitrogen Copper | [NAME] 0.23 (0.24 - cold roll forming) [NAME] 0.60 max 1.70 max 0.040 max 0.040 max 0.014 [NAME] 0.60 |  | [NAME] 0.45 |  | <16mm >16mm | 51 50 | 355 345 | [NAME] | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | >3mm 5,65√S0 4√S0 | 22 25 | 20 23 |  | 0 (32) |  | 27 (20) | 18.9
M10012 | C | M120 Y-04, rev 2 06/07 | EN 10210-1 | [NAME] | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Hot finished tubululars | t<25mm | EN 10204 Type 2.2 or higher | Hot finished. seamless hollow sections with wall thickness >10 mm accelerated cooling (DC) or quenched and tempered (QT) | Carbon Silicon Manganese Phosphorus Sulfur Nitrogen | [NAME] 0.22 max 0.55 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 | P:      N: | For each decrease of 0.005%, N [NAME] may be increased by 0.001% up to 0.012%.  Does not apply if a minimum total AL of 0.020% with a minimum Al/N ratio of 2:1can be shown. | Carbon Silicon Manganese Phosphorus: Sulfur: [NAME]: | [NAME] 0.25 [NAME] 0.60 max 1.70 [NAME] 0.045 [NAME] 0.045 [NAME] 0.011 | t<16 t>16 | [NAME] 0.45 [NAME] 0.47 |  | t<16 16<t<25 | 51 50 | 355 345 | [NAME] 3<t<25 | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | 5,65√S0 4√S0 | 22 25 | 20 23 |  | 0 (32) |  | 27 (20) | 18.9
M10012 | C | M120 Y-04, rev 2 06/07 | EN 10219-1 | S355J2H | SQL IV  S355 grade steel of SQL III, II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars | t<25mm | EN 10204 Type 3.1 or higher | as rolled or normalized/normalized rolled (N) followed by cold forming. | Carbon Silicon Manganese Phosphorus Sulfur | [NAME] 0.22 max 0.55 [NAME] 1.60  max 0.030 [NAME] 0.030 |  |  | Carbon Silicon Manganese Phosphorus Sulfur | [NAME] 0.24 max 0.60 max 1.70 max 0.040 max 0.040 |  | [NAME] 0.45 |  | <16mm >16mm | 51 50 | 355 345 | [NAME] | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | t>3mm: 5,65√S0 4√S0  Other dim and shapes for 5,65√S0: D/T<15 (round) and B+H)/2T<12.5 [NAME] | 20        18 17 | 23 |  | -20 (-4) |  | 27 (20) | 18.9
 |  |  | EN 10025-5 | S355J0WP |  | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher |  | C Si Mn P S N Cr Cu Ni N binding elem: Al Nb V Ti | [NAME] 0.12 max 0.75 max 1.0 0.06 - 0.15 max 0.035 [NAME] 0.009 0.30 - 1.25 0.25 - 0.55 max 0.65  min 0.020 0.015 - 0.060 0.02 - 0.12 0.02 - 0.10 | N: Does not apply if Al tot | min 0.020% | C Si Mn P S N Cr Cu Ni N binding elem: Al Nb V Ti | [NAME] 0.15 max 0.80 [NAME] 1.1 0.05 - 0.16 max 0.040 [NAME] 0.010 0.25 - 1.35 0.20 - 0.60 [NAME]  min 0.020 0.010 - 0.065 0.01 - 0.14 0.01 - 0.12 |  | [NAME] 0.52 |  | <16mm >16mm | 51 50 | 355 345 | <3[NAME]  flat prod: 3<t<12 long prod: >3mm | 74 - 98    68 - 91 | 510 - 680    470 - 630 |  |  |  |  | [NAME]1.5<t<2 2<t<2.5 2.5<t<3  L0=5.65√S0 flat prod: 3<t<12 long prod: >3mm | 16 17 18    22 | 14 15 16    20 |  | 0 |  | 27 | 18.9
 |  |  | EN 10025-5 | S355J0W |  | Plates and sections | t<25mm | EN 10204 Type 2.2 or higher |  | C Si Mn P S N Cr Cu Ni Mo Zr N binding elem: Al Nb V Ti | [NAME] 0.16 [NAME] 0.50 0.50 - 1.50 [NAME] 0.035 [NAME] 0.035 [NAME] 0.009 0.40 - 0.80 0.25 - 0.55 max 0.65 [NAME] 0.30 [NAME] 0.15  min 0.020 0.015 - 0.060 0.02 - 0.12 0.02 - 0.10 | N: Does not apply if Al tot | min 0.020% | C Si Mn P S N Cr Cu Ni Mo Zr N binding elem: Al Nb V Ti | [NAME] 0.19 [NAME] 0.55 0.45 - 1.60 max 0.040 max 0.040 [NAME] 0.010 0.35 - 0.85 0.20 - 0.60 [NAME] 0.70 [NAME] 0.35 max 0.17  min 0.020 0.010 - 0.065 0.01 - 0.14 0.01 - 0.12 |  | [NAME] 0.52 |  | <16mm >16mm | 51 50 | 355 345 | [NAME] | 74 - 98 68 - 91 | 510 - 680 470 - 630 |  |  |  |  | [NAME]1.5<t<2 2<t<2.5 2.5<t<3  L0=5.65√S0 t>3 | 16 17 18   22 | 14 15 16   20 |  | 0 |  | 27 | 18.9
M10015 | E | M-120 Y-08, rev 3 06/07 | EN 10219-1 | S355MLH | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars. | t<25mm | EN 10204 Type 3.1 or higher | Thermomechanically rolled (M) followed by cold forming. | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Aluminium Titianium Nickel Molybdenum Nitrogen | [NAME] 0.16 [NAME] 0.50 [NAME] 0.025 max 0.015 [NAME] 0.050 [NAME] 0.10 total min 0.020 [NAME] 0.050 [NAME] 0.30 max 0.20 max 0.020 | [NAME] | If sufficient N binding elements are present, the minimum Al content does not apply. The total sum of Cr, Cu and Mo shall not be higher than 0.60%. | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Aluminium Titianium Nickel Molybdenum Nitrogen | [NAME] 0.16 max 0.55 1.45 - 1.60 max 0.025 max 0.015 [NAME] 0.060 [NAME] 0.12 total min 0.015 [NAME] 0.060 [NAME] 0.55 max 0.23 max 0.022 |  | [NAME] 0.43 |  | <16mm >16mm | 51 50 | 355 345 | >3mm | 65 - 88 | 450 - 610 |  |  |  |  | 5,65√S0 4√S0 | 22 25 |  |  | -50 (-58) |  | 27 (20.5) | 19 (14) |  |  |  |  |  |  |  |  |  |  | The surface of the material shall comply to rust grade A or rust grade B or better according to ISO 8501-1. |  | The products shall be suitable for hot dip galvanizing
M10015 | C | M120 Y-08, rev 3 06/07 | EN 10219-1 | S355MLH | SQL III  S355 grade steel of SQL II or I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Cold formed tubulars. | t<25mm | EN 10204 Type 3.1 or higher | by cold forming. | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Aluminium Titianium Nickel Molybdenum Nitrogen | [NAME] 0.16 [NAME] 0.50 [NAME] 0.025 max 0.015 [NAME] 0.050 [NAME] 0.10 total min 0.020 [NAME] 0.050 [NAME] 0.30 max 0.20 max 0.020 | [NAME] | If sufficient N binding elements are present, the minimum Al content does not apply. The total sum of Cr, Cu and Mo shall not be higher than 0.60%. | Carbon Silicon Manganese Phosphorus Sulfur Niobium Vanadium Aluminium Titianium Nickel Molybdenum Nitrogen | [NAME] 0.16 max 0.55 1.45 - 1.60 max 0.025 max 0.015 [NAME] 0.060 [NAME] 0.12 total min 0.015 [NAME] 0.060 [NAME] 0.23 max 0.022 |  | [NAME] 0.43 |  | <16mm >16mm | 51 50 | 355 345 |  | 65 - 88 | 450 - 610 |  |  |  |  | 5,65√S0 4√S0 | 22 25 |  |  | -50 (-58) |  | 27 (20.5) | 18.9
M10016 | E | M-120 Y20, rev 5 06/07 | EN 10225 | S355G10+N | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and Z qual | t<150[NAME]  thicker materials may be accepted after concession request if all requirements in EN S355G10+N/ G10+M and NORSOK MDS Y-20 are documented. | EN 10204 Type 3.1 or higher | N: Normalized  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME] | As  Sb Sn Pb Bi Ca B | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005 | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N  Max. [NAME]. Elem. As  Sb Sn Pb Bi Ca B | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME]   0.03  0.010 0.020  0.010 0.010  0.005 0.0005 |  |  | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 | >54.4 >53.6 | >376 >368 | <16mm >16mm | 0.87 0.85 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) | t>12.5mm | 50 (35)  Strain Aged:  36 | 35 (24.5)    26 | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10016 | E | M-120 Y20, rev 5 06/07 | EN 10225 | [NAME] | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and Z qual | t<100[NAME]  thicker materials may be accepted after concession request if all requirements in EN S355G10+N/ G10+M and NORSOK MDS Y-20 are documented. | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME]2:1 | As  Sb Sn Pb Bi Ca B | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005 | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 max 0,08 | t<75mm t>75[NAME] |  | [NAME] 0.21 [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 | 51 51 50 49 47 | 355 355 345 335 325 | <100 | 68-91 | 470-630 | >54.4 | >376 | <16mm >16mm | 0.93 0.90 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) | t>12.5mm | 50  Strain Aged:  36 | 35    26 | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10016 | E |  |  | TTSTE S355 Z3 ([NAME]: Miras)  -without concession request |  | Plates and Z qual | [NAME] | EN 10204 Type 3.1 or higher |  | C | [NAME] 0.14 |  |  |  |  |  |  | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 | >54.4 >53.6 | >376 >368 |  |  | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) | t>12.5mm | 50 (35)  Strain Aged:  36 | 35 (24.5)    26 | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10016 | C | M120 Y20, rev 5 06/07 | EN 10225 | S355G10+N | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and Z qual | t<150[NAME]  thicker matr, may be accep. with concess. request | EN 10204 Type 3.1 or higher | N: Normalized  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME] | As  Sb Sn Pb Bi Ca B | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005 | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME] |  | [NAME] 0,43 | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 | >54.4 >53.6 | >376 >368 | <16mm >16mm | 0.87 0.85 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) |  | 50 (35) | 35 (24.5) | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5 | [NAME]: t>12.5mm |  | 36 | 26
M10016 | C | M120 Y20, rev 5 06/07 | EN 10225 | [NAME] | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates and Z qual | t<100[NAME]  thicker matr, may be accep. with concess. Request | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti  Al:N | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 [NAME]2:1 | As  Sb Sn Pb Bi Ca B | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005 | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,015 [NAME] 0,005 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0,06 max 0,08 | t<75mm t>75[NAME] | [NAME] 0,42 | [NAME] 0.21 [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 | 51 51 50 49 47 | 355 355 345 335 325 | <100 | 68-91 | 470-630 | >54.4 | >376 | <16mm >16mm | 0.93 0.90 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) |  | 50 (35) | 35 (24.5) | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5 | [NAME]: t>12.5mm |  | 36 | 26
M10016 | C |  |  | TTSTE S355 Z3 ([NAME]: Miras)  -without concession request |  | Plates and Z qual | [NAME] | EN 10204 Type 3.1 or higher |  | C | [NAME] 0.14 |  |  |  |  |  |  | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 | >54.4 >53.6 | >376 >368 |  |  | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) |  | 50 (35) | 35 (24.5) | [NAME]  (piling matr. Test temp: -30) | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5 | [NAME]: t>12.5mm |  | 36 | 26
M10017 | E | M120 Y25 rev 5 06/07 | EN 10225 | S355G9+N | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | t<150[NAME] | EN 10204 Type 3.1 or higher | N: Normalized  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 |  |  | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 |  |  | <16mm >16mm | 0.87 0.85 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) | t>12.5mm | 50 (35)  Strain Aged:  36 | 35 (24.5)    26 |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10017 | E | M120 Y25 rev 5 06/07 | EN 10225 | S355G9+M | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | t<100[NAME] | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 |  |  | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 | 51 51 50 49 47 | 355 355 345 335 325 | <100 | 68-91 | 470-630 |  |  | <16mm >16mm | 0.93 0.90 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) | t>12.5mm | 50 (35)  Strain Aged:  36 | 35 (24.5)    26 |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10017 | C | M120 Y25, rev 5 06/07 | EN 10225 | S355G9+N | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | t<150[NAME] | EN 10204 Type 3.1 or higher | N: Normalized  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  Si Mn P  S  Cr Mo Ni  t<40mm [NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME][NAME] 0,70 max 0,30 0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 |  | [NAME] 0,43 | [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 100<t<150 | 51 51 50 49 47 46 | 355 355 345 335 325 320 | <100 >100 | 68-91 67-90 | 470-630 460-620 |  |  | <16mm >16mm | 0.87 0.85 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 (35) | 35 (24.5) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5 | [NAME]: t>12.5mm |  | 36 | 26
M10017 | C | M120 Y25, rev 5 06/07 | EN 10225 | S355G9+M | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | t<100[NAME] | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered also accepted | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  Si Mn P  S  Cr Mo t<75mm t>75[NAME] (total) Cu  N  Nb  Ti  V  Nb+V  Nb+V+Ti | [NAME] [NAME] 1,65 [NAME] 0,020 [NAME] 0,010 [NAME] 0,20  [NAME] 0,20  [NAME]0.015 - 0.055 [NAME] 0,010 max 0,030 max 0,025 [NAME] 0,060 max 0.06 max 0,08 | t<75mm t>75[NAME] | [NAME] 0,42 | [NAME] 0.21 [NAME] 0.22 | <16 16<t<25 25<t<40 40<t<63 63<t<100 | 51 51 50 49 47 | 355 355 345 335 325 | <100 | 68-91 | 470-630 |  |  | <16mm >16mm | 0.93 0.90 | 5,65√S0 4√S0 | 22 25 |  |  | -40 (-40) |  | 50 (35) | 35 (24.5) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5 | [NAME]: t>12.5mm |  | 36 | 26
M10021 | E | M-120 Y41, rev 5 06/07 | EN 10225 | S460G4+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | M: Thermo-mechanically rolled  Quenched and tempered may also be accepted (Q, QT) | C  Si  Mn  P  S  Cr  Mo  Ni Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME] 0,7 0.015 - 0,055 max 0,3 [NAME] 0,012 max 0,05 [NAME] 0,025 [NAME] 0,8 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1  These elements shall be checked at least once every 5000 tonnes at each manufacturing location and shall be reported as a cast analysis. | C  Si  Mn P  S  Cr  Mo  Ni  Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME] 0,7 0.015 - 0,055 max 0,3 [NAME] 0,012 max 0,05 [NAME] 0,025 [NAME] 0,8 [NAME] |  |  | [NAME] 0.24 |  | 66,5 - 84 | 460 - 580 |  | 79,5 - 101,5 | 550 - 700 |  | 440 | >16mm | 0.9 | 5,65√S0 4√S0 | 17 19 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 60 (44) 60 (44) | 42 (31) 42 (31) |  | 10mmx7.5mm 10mmx5mm | 45 30 | 31.5 21 |  |  | as agreed | as agreed
M10021 | C | M120 Y41, rev 5 06/07 | EN 10225 | S460G4+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | M: Thermo-mechanically rolled  Quenched and tempered may also be accepted (Q, QT) | C Si Mn P S Cr Mo Ni  Al (total) Cu N  Nb Ti  V  Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME] 0,7 0.015 - 0,055 max 0,3 [NAME] 0,012 max 0,05 [NAME] 0,025 [NAME] 0,8 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C Si Mn P S Cr Mo Ni  Al (total) Cu N  Nb Ti  V  Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME] 0,7 0.015 - 0,055 max 0,3 [NAME] 0,012 max 0,05 [NAME] 0,025 [NAME] 0,8 [NAME] |  |  | [NAME] 0.24 |  | 66.5 - 84 | 460 - 580 |  | 79.5 - 101.5 | 550 - 700 |  | 440 | >16mm | 0.90 | 5,65√S0 4√S0 | 17  19 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 60 (44) | 42 (31) |  | 10mmx7.5mm 10mmx5mm | 45 30 | 31.5 21 |  |  | as agreed | as agreed
M10022 | E | M120 Y21, rev 5 06/07 | EN 10225 | S355G12+N S355G12+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections | <63mm | EN 10204 Type 3.1 or higher | N: Normalized M: Termo-mechanically rolled | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.020 [NAME] 0.007 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 |  |  |  |  | [NAME] 0.24 | <16mm 16-40mm 40-63mm | 51 50 22 | 355 345 335 |  |  | 460 - 620 |  | 368 |  | 0.87 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -20 -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10022 | C | M120 Y21, rev 5 06/07 | EN 10225 | S355G12+N S355G12+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections | <63mm | EN 10204 Type 3.1 or higher | N: Normalized M: Termo-mechanically rolled | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.020 [NAME] 0.007 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 |  |  |  |  | [NAME] 0.24 | <16mm 16-40mm 40-63mm |  | 355 345 335 |  |  | 460 - 620 |  | 368 |  | 0.87 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10023 | E | M120 Y22, rev 5 06/07 | EN 10225 | S355G15+Q S355G15+N | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Seamless tubulars and hollow sections |  | EN 10204 Type 3.1 or higher | N: Normalized/normalized rolled  Q or QT: Quenched and tempered | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.16  0.15 - 0.55 [NAME] 1.60 max 0.025 max 0.007 [NAME] 0.25 [NAME] 0.08 [NAME] 0.30  max 0.06 [NAME] 0.35 [NAME] 0.014 [NAME] 0.050 max 0.02 [NAME] 0.10 max 0.80 [NAME] 0.10 max 0.12 | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 |  |  |  | [NAME] 0.43 |  | <20mm 20<t<40 |  | 355 345 |  |  | 460 - 620 |  | 368 |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10023 | C | M120 Y22, rev 5 06/07 | EN 10225 | S355G15+Q S355G15+N | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Seamless tubulars and hollow sections |  | EN 10204 Type 3.1 or higher | N: Normalized/normalized rolled  Q or QT: Quenched and tempered | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.16  0.15 - 0.55 [NAME] 1.60 max 0.025 max 0.007 [NAME] 0.25 [NAME] 0.08 [NAME] 0.30  max 0.06 [NAME] 0.35 [NAME] 0.014 [NAME] 0.050 max 0.02 [NAME] 0.10 max 0.80 [NAME] 0.10 max 0.12 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 |  |  |  | [NAME] 0.43 |  | <20mm 20<t<40 |  | 355 345 |  |  | 460 - 620 |  | 368 |  | 0.88 | 5,65√S0 4√S0 | 22 25 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10024 | D | M120 Y26, rev 5 06/07 | EN 10225 | S355G11+N  S355G11+M | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | N: Normalized / normalized rolled  M: Thermo-mechanically rolled | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.025 max 0.015 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.025 max 0.015 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 |  |  | [NAME] 0.24 | t<16 16<t<40 40<t<63 | 51 50 48.5 | 355 345 335 |  | 67 - 90 | 460 - 620 |  |  |  | 0.87 | 5,65√S0 | 22 |  |  | -20 (-4) -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10024 | B | M120 Y26, rev 5 06/07 | EN 10225 | S355G11+N  S355G11+M | SQL II   S355 grade steel of SQL I may be supplied without a concession request to FMC.  Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | N: Normalized / normalized rolled  M: Thermo-mechanically rolled | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.025 max 0.015 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | Carbon  Silicon Manganese Phosphorus Sulfur Cromium Molybdenum Nickel Aluminium Copper Nitrogen Niobium Titanium  Vanadium Cr+Mo+Ni+Cu Nb+V  Nb+V+Ti | [NAME] 0.14  max 0.55 [NAME] 1.65 [NAME] 0.025 max 0.015 [NAME] 0.25 [NAME] 0.08 [NAME] 0.50  0.015 - 0.055 [NAME] 0.30 [NAME] 0.012 [NAME] 0.040 [NAME] 0.025 [NAME] 0.060 [NAME] 0.80 max 0.06 [NAME] 0.08 |  |  | [NAME] 0.24 | t<16 16<t<40 40<t<63 | 51 50 48.5 | 355 345 335 |  | 67 - 90 | 460 - 620 |  |  |  | 0.87 | 5,65√S0 | 22 |  |  | -20 (-4) -40 (-40) | [NAME] | 50 (35) | 35 (24) |  | 10mmx7.5mm 10mmx5mm | 37.5 25 | 26.25 17.5
M10025 | E | M120 Y30, rev 5 06/07 | EN10225 | S420G2+QT / S420G2+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | 100mm | EN 10204 Type 3.1 or higher | Q or QT: quenched & tempered  M: Thermo-mechanically rolled | C  -t>15mm -t<15[NAME] (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,020 [NAME] 0,007 max 0,25 max 0,25 [NAME]0,015 - 0,055 [NAME] 0,010 max 0,040 max 0,025 max 0,080 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 | C  -t>15mm -t<15[NAME] (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,020 [NAME] 0,007 max 0,25 max 0,25 [NAME]0,015 - 0,055 [NAME] 0,010 max 0,040 max 0,025 max 0,080 [NAME] | [NAME] t>15[NAME] | 0,42 | [NAME] 0.23 [NAME] |  | 61 - 78 | 420 - 540 |  | 72 - 96 | 500 - 660 | 57.6 | 400 | [NAME] | 0,93 0,90 | 5,65√S0 4√S0 | 19 22 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) | [NAME]: t>12.5mm | 60 (44)    42 | 42 (30,8)    26 | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4)
M10025 | C | M120 Y30, rev 5 06/07 | EN10225 | S420G2+QT / S420G2+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | 100mm | EN 10204 Type 3.1 or higher | Q: quenched & tempered  M: Thermo-mechanically rolled | C  -t>15mm -t<15[NAME] (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,020 [NAME] 0,007 max 0,25 max 0,25 [NAME]0,015 - 0,055 [NAME] 0,010 max 0,040 max 0,025 max 0,080 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  -t>15mm -t<15[NAME] (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,020 [NAME] 0,007 max 0,25 max 0,25 [NAME]0,015 - 0,055 [NAME] 0,010 max 0,040 max 0,025 max 0,080 [NAME] | [NAME] t>15[NAME] | 0.42 | [NAME] 0.23 [NAME] |  | 61 - 78 | 420 - 540 |  | 72 - 96 | 500 - 660 | 57.6 | 400 | [NAME] | 0,93 0,90 | 5,65√S0 4√S0 | 19 22 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) |  | 60 (44) | 42 (30.8) | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4) | [NAME]: t>12.5mm |  | 42 | 26
M10026 | E | M120 Y31, rev 5 06/07 | EN 10225 | S420G4+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered & normalized may also be accepted | C  Si Mn P  S  Cr  Mo  Ni  Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME]0.015 - 0,055 [NAME] 0,012 max 0,050 [NAME] 0,025 max 0,080 max 0,80 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 | C  Si Mn P  S  Cr  Mo  Ni  Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME]0.015 - 0,055 [NAME] 0,012 max 0,050 [NAME] 0,025 max 0,080 max 0,80 [NAME] |  |  | [NAME] |  | 61 - 78 | 420 - 540 |  | 72 - 96 | 500 - 660 | 57.6 | 400 |  | 0.90 | 5,65√S0 4√S0 | 19 22 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 60 (44) 60 (44) | 42 (30,8) 42 (30,8) | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4) |  |  | as agreed | as agreed
M10026 | C | M120 Y31,  rev 5 06/07 | EN 10225 | S420G4+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Rolled sections |  | EN 10204 Type 3.1 or higher | M: Thermo mechanically rolled.  Quenched & tempered & normalized may also be accepted | C  Si Mn P  S  Cr  Mo  Ni  Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME]0.015 - 0,055 [NAME] 0,012 max 0,050 [NAME] 0,025 max 0,080 max 0,80 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C  Si Mn P  S  Cr  Mo  Ni  Al (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 [NAME]0.015 - 0,055 [NAME] 0,012 max 0,050 [NAME] 0,025 max 0,080 max 0,80 [NAME] |  |  | [NAME] |  | 61 - 78 | 420 - 540 |  | 72 - 96 | 500 - 660 | 57.6 | 400 |  | 0.90 | 5,65√S0 4√S0 | 19 22 |  | Z-testing Av: 35 Sing: 25 | -20 (-4) -40 (-40) | [NAME] | 60 (44) | 42 (30.8) | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4) |  |  | as agreed | as agreed
M10027 | D | M120 Y40, rev 5 06/07 | EN 10225 | S460G2+QT / S460G2+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | 100mm | EN 10204 Type 3.1 or higher | QT: Quenched and tempered  M: Thermo mechanically rolled | C -t>15mm -t<15[NAME] (total) Cu  N  Nb  Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,15 max 0,15 - 0,55 max1,65 max 0,02 [NAME] 0,007 max 0,25 max 0,25 [NAME] 0,7 0,015 - 0,055 max 0,3 [NAME] 0,04 [NAME] 0,025 [NAME] 0,9 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | 0.03  0.010 0.020  0.010 0.010  0.005 0.0005  2:1 | C -t>15mm -t<15[NAME] (total) Cu  N  Nb Ti  V  Cr+Mo+Ni+Cu  Nb+V  Nb+V+Ti | [NAME] 0,14 [NAME] 0,15 max 0,15 - 0,55 max1,65 max 0,02 [NAME] 0,007 max 0,25 max 0,25 [NAME] 0,7 0,015 - 0,055 max 0,3 [NAME] 0,04 [NAME] 0,025 [NAME] 0,9 [NAME] | t<15 t<15 |  | [NAME] 0.23 [NAME] 0.22 |  | 66.5 - 84 | 460 - 580 |  | 79.5 - 101.5 | 550 - 700 |  | 400 | [NAME] | 0,93 0,90 | 5,65√S0 4√S0 | 17 19 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) | Strain Aged: [NAME] | 60 (44)   46 | 42 (31)   29 | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4)
M10027 | B | M120 Y40, rev 5 06/07 | EN 10225 | S460G2+QT / S460G2+M | SQL I   Materials certified to other industrial standards may be used if the minimum req. are fulfilled, with a concession request accepted by FMC. | Plates | 100mm | EN 10204 Type 3.1 or higher | Q: Quenched  M: Thermo mechanically rolled | C -t>15mm -t<15[NAME] (total) Cu N  Nb Ti  V  Cr+Mo+Ni+Cu  Nb+V Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 max 0,25 [NAME] 0,7 0,015 - 0,055 max 0,3 [NAME] 0,04 [NAME] 0,025 [NAME] 0,9 [NAME] | As  Sb Sn Pb Bi Ca B  Al:N | [NAME] 0.03  [NAME] 0.010 max 0.020  [NAME] 0.010 [NAME] 0.010  max 0.005 [NAME] 0.0005  2:1 | C -t>15mm -t<15[NAME] (total) Cu N  Nb Ti  V  Cr+Mo+Ni+Cu  Nb+V Nb+V+Ti | [NAME] 0,14 max 0,15 0,15 - 0,55 [NAME] 1,65 [NAME] 0,02 [NAME] 0,007 max 0,25 max 0,25 [NAME] 0,7 0,015 - 0,055 max 0,3 [NAME] 0,04 [NAME] 0,025 [NAME] 0,9 [NAME] | [NAME] t>15mm | 0.43 | [NAME] 0.23 [NAME] 0.22 |  | 66.5 - 84 | 460 - 580 |  | 79.5 - 101.5 | 550 - 700 | 57.6 | 400 | [NAME] | 0,93 0,90 | 5,65√S0 4√S0 | 17 19 |  | Z-testing Av: 35 Sing: 25 | -40 (-40) |  | 60 (44) | 42 (30.8) | [NAME] | 10mmx7.5mm 10mmx5mm | 45 (33) 30 (22) | 31.5 (23) 21 (15.4) | [NAME]: t>12.5mm |  | 46 | 29
M11799 | C |  | MDS-[PHONE] | S355 Carbon steel |  | plates, beams, channels, angles, bar, tube ...etc. | <100mm | EN 10204 Type 3.1 or higher | normalised/normalised rolled (+N) | C Mn P S V+Nb | [NAME] 0.20 max 1.70 [NAME] 0.035 [NAME] 0.030 max 0.12 |  |  |  |  |  | [NAME] 0.45 |  | <16mm 16-40mm 40-63mm 63-80mm 80-100mm | 51 50 49 47 46 | 355 345 335 325 315 | <100mm | 68 - 91 | 470 - 630 |  |  |  |  |  | 20 |  |  | -20 | t<150 | 27 | 18.9